Using MATLAB to Design and Analyse Composite Laminates


 Anissa Simmons
 1 years ago
 Views:
Transcription
1 Engineering, 2010, 2, doi: /eng Published Online November 2010 ( Using MATLAB to Design and Analyse Composite Laminates Abstract Avinash Ramsaroop, Krishnan Kanny * Department of Mechanical Engineering, Durban University of Technology, Durban, South Africa Received July 3, 2010; revised August 5, 2010; accepted August 19, 2010 This work deals with the generation of MATLAB script files that assists the user in the design of a composite laminate to operate within safe conditions. The inputs of the program are the material properties, material limits and loading conditions. Equations based on Hooke s Law for twodimensional composites were used to determine the global and local stresses and strains on each layer. Failure analysis of the structure was performed via the TsaiWu failure theory. The output of the program is the optimal number of fibre layers required for the composite laminate, as well as the orientation of each layer. Keywords: Composite Laminates, Hooke s Law, Fibre Angle, MATLAB, Composite Design 1. Introduction Composites are etremely versatile materials and may be tailored to suit any function. They have found uses from the aerospace industry to common everyday applications. However, one drawback of these materials is tedious design processes [1]. Therefore, in an attempt to reduce this time consuming phase, it was decided to develop a computer program that assisted the user in designing a composite structure. The program needed to perform the necessary calculations in the fraction of the time it would take if done using conventional techniques. Conventional methods for designing composite structures involve the use of Hooke s law for twodimensional unidirectional composites. Equations relating the stresses and strains in these materials have been developed and are available from various tets [24]. These equations, however, are limited to flat unidirectional laminates. The procedure to follow is quite laborious. The material properties, material limits, number of fibre layers, and the fibre orientation and thickness of each layer as well as the loading conditions need to be known. These quantities are then used in the governing equations and numerous matri computations are required. The outputs from these equations are the global and local stresses and strains of each layer. The local stresses on each layer are then compared to the allowable material limits and, if they eceed these limits, the entire process needs to be repeated with new angles and, if necessary, more fibre layers. If a composite structure has to be designed to optimally carry the applied loads, the manual calculations would take an etremely long time. Designers usually use standard fibre angles in their design to overcome the time factor because eact fibre orientation is diffic [5]. As a res composite structures are usually overdesigned as incorrect fibre angles may mean more fibre layers which in turn leads to increased material costs. Many researchers [69] have attempted to reduce material costs by reducing the laminate thickness but these were based on fied fibre angles. Certain regions of a composite structure, such as holes and other high stress zones, may need more reinforcement than others. Only these areas would require more fibre layers. However, with the conventional approach to design, the entire structure would be laid up to compensate for the high stress concentrations which increases the material costs. Therefore an approach was needed where the calculations can be performed easily and automatically, and where only the regions with high stresses have etra reinforcement. A logical solution was to write computer programs to perform the computations. MATLAB, a numerical computing package, was used as a basis for the programs as it is more than sufficient to handle the numerous matri computations [1014]. It may also be interfaced with programs written in other languages, such as C, C++, and FORTRAN [1314]. Basically, two programs were generated and each program consisted of a main script file and various functions. The first program was written according to the conventional methods for designing composite structures. The purpose of this program was to determine whether its
2 A. RAMSAROOP ET AL. 905 functions operated efficiently and performed calculations correctly as these would be used for the second program. Ress from this program were compared to manually calculated eamples. The second program used a different approach where the number of inputs were reduced to just the material properties, material limits and applied loading conditions. The outputs of this program are the number of layers and the fibre angle of each layer. These programs are discussed in further detail after the equations governing the stressstrain relationships are eamined. 2. Hooke s Law for TwoDimensional Composite Structures Figure 1 shows a schematic representation of a composite lamina. The direction along the fibre ais is designated 1. The direction transverse to the fibre ais but in the plane of the lamina is designated 2. The direction transverse to both the fibre ais and the plane of the lamina (out of page) is designated 3. This direction is not shown in the figure as it only becomes necessary in threedimensional cases. The 12 coordinate system can be considered to be local coordinates based on the fibre direction. However this system is inadequate as fibres can be placed at various angles with respect to each other and the structure. Therefore a new coordinate system needs to be defined that takes into account the angle the fibre makes with its surroundings. This new system is referred to as global coordinates (y system) and is related to the local coordinates (12 system) by the angle θ. A composite material is not isotropic and therefore its stresses and strains cannot be related by the simple Hooke s Law ( E ). This law has to be etended to twodimensions and redefined for the local and global coordinate systems [2]. The res is Equations (1) and (2). Figure 1. Global coordinate system in relation to local coordinate system. Q Q Q12 Q Q Q11 Q12 Q 16 y Q12 Q22 Q26 y y Q16 Q26 Q 66 y where σ 1,2 are the normal stresses in directions 1 and 2; τ 12 is the shear stress in the 12 plane; ε 1,2 are the normal strains in directions 1 and 2; γ 12 is the shear strain in the 12 plane; [Q] is the reduced stiffness matri; σ,y are the normal stresses in directions and y; τ y is the shear stress in the y plane; ε,y are the normal strains in directions and y; γ y is the shear strain in the y plane; [ Q ] is the transformed reduced stiffness matri. The elements of the [Q] matri in Equation (1) are dependent on the material constants and may be calculated using Equation (3). E E E Q, Q, Q, Q G (1) (2) (3) where E 1,2 are Young s modulus in directions 1 and 2; G 12 is the shear modulus in the 12 plane; ν 12,21 are Poisson s ratios in the 12 and 21 planes. The [ Q ] matri in Equation (2) may be determined by Equation (4). 1 1 Q T QRTR (4) where [T] is the transformation matri; [R] is the Reuter matri. These matrices are given by: 2 2 c s 2sc T s c 2sc and R (5) 2 2 sc sc c s where c = cosθ; s = sinθ. The local stresses and strains in Equation (1) are related to the global stresses and strains in Equation (2) by Equation (6) y T 2 and 2 RTR y y y Equations (1) to (6) are used to determine the stresses and strains for a single composite layer. Since composites are milayered entities, equations for this case must also be set up. The res is Equation (7). 0 N A B M B D (7) (6)
3 906 A. RAMSAROOP ET AL. where N is the vector of resant forces; M is the vector of resant moments; ε 0 is the vector of the midplane strains; κ is the vector of midplane curvatures. Vectors ε and κ are related to the global coordinates by Equation (8). 0 0 y y z y (8) 0 y y y where z is an arbitrary distance from the midplane. The [A], [B], and [D] matrices in Equation (7) are known as the etensional, coupling, and bending stiffness matrices, respectively. The elements of these matrices may be determined from Equations (9) to (11). n 1 A Q h h i 1, 2, 3 j 1, 2, 3 (9) ij ij k k k 1 k n 1 B Q h h i 1, 2, 3 j 1, 2, 3 (10) ij ij k k 2 k 1 k n 1 Dij Qij hk hk i 1, 2, 3 j 1, 2, 3 (11) 3 k 1 k where n is the number of layers; Qij is the ith, k jth element of the [ Q ] matri of the kth layer; h k is the distance of the top or bottom of the kth layer from the midplane of the composite. Figure 2 illustrates how to determine the distance h k from the midplane. The final aspect involved in the design of a composite structure is the failure analysis. There are various failure theories; however, the TsaiWu failure criterion is only one that closely correlates with eperimental data. This failure theory is given by Equation (12). H H H H H H 2H (12) The parameters for the TsaiWu failure criterion are given by Equation (13) H1 ; H2 ; H6 0 T C T C H11 ; H22 ; H66 T C T C H12 T C T C (13) T where 12, are the imate tensile stresses in direction 1 and 2; 12, are the imate compressive C stresses in direction 1 and 2; 12 is the imate shear stress in the 12 plane. In order to better facilitate the use of this failure theory, each stress component of Equation (12) was miplied by a variable [2]. This variable is referred to as the strength ratio (SR) and combining this in Equation (12) resed in Equation (14). ( H11 H22 H612) SR (14) ( H111 H222 H H1212 ) SR 1 The purpose of SR is to directly determine by what ratio the local stresses must be increased or decreased to avoid failure. This also directly relates to the applied forces. The criterion for SR is that it can only be positive. If SR is less than 1, then failure occurs because it means that the loading needs to decrease to avoid failure. A SR value of 1 implies that the composite structure is perfectly suited for the applied loading conditions. A value of greater than 1 means that the structure is more than capable of carrying the applied loading and that the loading may also be increased. For eample, a SR value of 1.5 means that the loading may be increased up to 50% without failure occurring. Figure 2. Locations of layers in a composite structure [2].
4 A. RAMSAROOP ET AL Programming 3.1. Conventional Approach Program This approach follows the commonly found methods laid out in the various tets [24]. As stated above, the material constants, material limits, number of fibre layers, fibre angle of each layer, and the thickness of each layer as well as the loading conditions need to be known. The following procedure illustrates the steps involved in this approach: 1) Calculate the [Q] matri for each layer using Equation (3). 2) Using Equation (5), compute the [T] matri for each layer. 3) Determine [ Q ] matri for each layer via Equation (4). 4) Find the location of the top and bottom surface of each layer, h k (k = 1 to n). 5) Use Equations (9), (10) and (11) to calculate the [A], [B], and [D] matrices. 6) Substitute these matrices as well as the applied loading into Equation (7) and solve the si simaneous equations to determine the midplane strains (ε 0 ) and curvatures (κ). 7) Find the global strains and stresses in each layer using Equations (8) and (2), respectively. 8) Find the local strains and stresses for each layer by using Equation (6). 9) Determine the parameters for the TsaiWu failure criterion via Equation (13). 10) Using these parameters and the local stresses for each layer, find SR via Equation (14). Once SR has been determined, the designer will know whether the structure will fail or not. If failure occurs, the fibre angles and possibly the number of layers have to be adjusted, and the above procedure needs to be repeated until no failure takes place. Manual calculations would take a long period, therefore a program was written to perform the necessary calculations. The program prompts the user for the following inputs: the material properties (E 1, E 2, G 12 and ν 12 ) the material limits ( T 1, C 1, T 2, C 2, 12 ) the number of layers (N) the fibre angle (θ) of each layer the thickness (t) of each layer applied loading conditions These input parameters were used to determine the [Q], [T], and [ Q ] matrices for each layer. All data concerning each layer (E 1, E 2, G 12, ν 12, θ, t, [Q], [T], and [ Q ]) were stored in an array. The data in this array was used to calculate the [A], [B], and [D] matrices. Using these matrices and the applied loading conditions, the global and local stresses and strains were computed. The local stresses were compared to the material limits, via the TsaiWu failure criterion, to determine whether the composite will fail. The computation of the various matrices and other relevant data was each carried out in a separate function. This means there was one function to determine the [Q] matri, another to calculate the [T] matri, and so on. A script file was written that controlled the use of each function. The purpose of the functions was to enable easier programming in future. This program was tested against manually calculated eamples in the various tets [2,3] and the ress were eactly comparable to the manual computations. In an eample (Eample 4.3) by Kaw [2], the stresses and strains in a graphite/epoy composite laminate were eamined. This laminate consisted of three layers, with fibre angles of 0, 30 and 45, and each layer had a thickness of 5 mm. The material properties, material limits and loading conditions used in this eample are given in Table 1. The resing global strains, global stresses, local strains and local stresses at the top, middle and bottom of each layer are shown in Figures 3 to 6, respectively. The values in Table 1 and the fibre angles of 0, 30 and 45 were used as inputs in the Conventional Approach script file. The global and local stresses and strains were computed and are shown in Figures 7 to 10. The values in these tables and the ones in Figures 3 to 6 are eactly comparable. The conclusion from this is that the Conventional Approach program can accurately determine the stresses and strains in a flat unidirectional composite structure. The Conventional Approach script file was further etended to include failure analysis via the TsaiWu failure theory. The resing SR values for the top, middle and bottom of each layer is shown in Figure 11. The rows represent the layers and columns 1 to 3 represent the top, middle and bottom of each layer, respectively. The SR values in Figure 11 indicate that the composite structure will fail first on layer 1 (SR = ) and then layer 2 (SR = ). It is clear from this that the input angles and number of layers were insufficient to carry the applied loads. Although this program performs all the relevant calculations easily and automatically, and significantly shortens the design process, using the program to design a composite structure would require much guesswork. The designer would enter the necessary input values, allow the program to perform the various calculations, and then discover whether the composite structure would fail. If failure does occur, as in the above case, the designer may have to change the fibre angles and/or the
5 908 A. RAMSAROOP ET AL. thickness of each layer and/or the number of layers. The choice of values may be uncertain and values would have to be assumed. Furthermore, it would also be an uncertainty on which values to change. Much time may be spent in achieving a structure that would not fail. On the other hand, if failure does not occur, the structure may prove to be overdesigned in which case the manufacturing costs of the structure may increase as unnecessary material will be used. To overcome these problems, a new script file was generated. Table 1. Material properties, limits and loading conditions for graphite/epoy composite eample in Kaw [2]. Material Properties Material Limits Forces Moments T C T C E 1 E 2 G ν (GPa) (GPa) (GPa) 12 (MPa) (MPa) (MPa) (MPa) (MPa) N M Table 4.1 Global Strains (m/m) in Eample 4.3 Ply # Position ε ε y γ y Top (10 8 ) (10 6 ) (10 6 ) 1 (0 o ) Middle (10 7 ) (10 6 ) (10 6 ) Bottom (10 7 ) (10 6 ) (10 6 ) Top (10 7 ) (10 6 ) (10 6 ) 2 (30 o ) Middle (10 7 ) (10 6 ) (10 7 ) Bottom (10 7 ) (10 6 ) (10 7 ) Top (10 7 ) (10 6 ) (10 7 ) 3 ( 45 o ) Middle (10 7 ) (10 6 ) (10 6 ) Bottom (10 7 ) (10 6 ) (10 6 ) Figure 3. Table from eample in Kaw [2] showing global strains. Table 4.2 Global Stresses (Pa) in Eample 4.3 Ply # Position y y Top (10 4 ) (10 4 ) (10 4 ) 1 (0 o ) Middle (10 4 ) (10 4 ) (10 4 ) Bottom (10 4 ) (10 4 ) (10 4 ) Top (10 4 ) (10 4 ) (10 4 ) 2 (30 o ) Middle (10 5 ) (10 4 ) (10 4 ) Bottom (10 5 ) (10 4 ) (10 4 ) Top (10 5 ) (10 5 ) (10 5 ) 3 ( 45 o ) Middle (10 4 ) (10 4 ) (10 4 ) Bottom (10 4 ) (10 4 ) (10 4 ) Figure 4. Table from eample in Kaw [2] showing global stresses. Table 4.3 Local Strains (m/m) in Eample 4.3 Ply # Position Top (10 8 ) (10 6 ) (10 6 ) 1 (0 o ) Middle (10 7 ) (10 6 ) (10 6 ) Bottom (10 7 ) (10 6 ) (10 6 ) Top (10 7 ) (10 6 ) (10 6 ) 2 (30 o ) Middle (10 7 ) (10 6 ) (10 6 ) Bottom (10 6 ) (10 6 ) (10 6 ) Top (10 6 ) (10 6 ) (10 6 ) 3 ( 45 o ) Middle (10 7 ) (10 6 ) (10 6 ) Bottom (10 7 ) (10 6 ) (10 7 ) Figure 5. Table from eample in Kaw [2] showing local strains.
6 A. RAMSAROOP ET AL. 909 Table 4.4 Local Stresses (Pa) in Eample 4.3 Ply # Position Top (10 4 ) (10 4 ) (10 4 ) 1 (0 o ) Middle (10 4 ) (10 4 ) (10 4 ) Bottom (10 4 ) (10 4 ) (10 4 ) Top (10 4 ) (10 4 ) (10 4 ) 2 (30 o ) Middle (10 5 ) (10 4 ) (10 4 ) Bottom (10 5 ) (10 4 ) (10 4 ) Top (10 5 ) (10 4 ) (10 4 ) 3 ( 45 o ) Middle (10 4 ) (10 4 ) (10 3 ) Bottom (10 4 ) (10 4 ) (10 3 ) Figure 6. Table from eample in Kaw [2] showing local stresses. Figure 7. Global strains from Conventional Approach program with Table 1 as inputs. Figure 8. Global stresses from Conventional Approach program with Table 1 as inputs.
7 910 A. RAMSAROOP ET AL. Figure 9. Local strains from Conventional Approach program with Table 1 as inputs. Figure 10. Local stresses from Conventional Approach program with Table 1 as inputs FibreAngleOutput Program Initially it was decided that this program should take the applied loading conditions, material properties and material limits as inputs. The program was to assume that the number of layers equals the number of input forces, and that the fibre angle of each layer equals the direction of each force. It would then perform all the necessary matri calculations as in the Conventional Approach. The global and local stresses and strains would be determined as before and failure analysis with the TsaiWu criterion may be performed. However, the assumptions made above cannot be used in a real situation as it may res in an overdesign of a composite structure as in the case of the conventional approach. Hence a program was written that does not make any assumptions but rather builds the laminate up one layer at a time. Basically this program varies the fibre angles to achieve a composite structure that is perfectly suited to carry the applied loading conditions. The
8 A. RAMSAROOP ET AL. 911 Figure 11. SR ratios from Conventional Approach program with Table 1 as inputs. outputs of the program are the number of layers and the fibre angle of each layer. The program asks the user to input the following: material properties material limits loading conditions The [Q] matri and the TsaiWu parameters can be calculated immediately as these do not vary with fibre angle but rather with material properties and limits. The program begins with one layer at an angle of 0 and computes h k, as well as the [T], [ Q ], [A], [B] and [D] matrices. Thereafter the midplane strains and curvatures, and, the global and local stresses and strains are calculated. The TsaiWu failure theory is applied and a value for SR is obtained for each layer. The program then analyzes the SR values and confirms whether it is in a certain range. The lower limit of this range is 1 as any value below this would mean failure. The upper limit in this range is 1.2 and this is to avoid overdesigning. If the SR value for each layer is between 1 and 1.2, then the design of the composite structure is complete. On the other hand, if the SR value for any of the layers is out of this range, the program varies that particular fibre angle to obtain a SR value between 1 and 1.2. However, due to the angle change all the matri calculations have to be redone. A new SR value is obtained for each layer and this is compared to the old values. If the new SR value for a particular layer is higher than the old SR value, then the angle of that layer is changed to the new one. For eample, after the initial calculation a layer with fibre angle of 30 has a SR value of 0.8. This is not acceptable and the program changes the angle to obtain a better SR value. Say at 35 the SR value is 0.9, the program will then change the angle of the 30 layer to 35. If at 35 the SR value was 0.7, then the program will retain the 30 angle. The program continues to change angles and compare old and new SR values until the SR value of each layer is between 1 and 1.2, in which case the design is completed. However, if this range cannot be achieved, a new layer is added on. The program starts from the beginning and recalculates the various matrices. SR values are obtained and the comparison between new and old values resumes. New layers will be added on until the SR value for each layer is between 1 and 1.2. The program then outputs the number of layers and the fibre angle of each layer. Figure 12 illustrates the procedure the script file follows to obtain the desired outputs. The FibreAngleOutput program was subjected to several runs. The ress, namely the number of layers and the fibre angles, needed to be verified. Therefore these were used as inputs in the Conventional Approach program. The TsaiWu failure theory was used and in each case there was no failure. As an eample, consider the graphite/epoy composite laminate eamined earlier. The material properties, material limits and loading conditions for this laminate were given in Table 1. The SR values for three layers with fibre angles of 0, 30 and 45 were shown in Figure 11. The values in Table 1
9 912 A. RAMSAROOP ET AL Obtain material properties and allowable limits Calculate [Q], [S] matrices Parameters for TsaiWu 5 4 Enter magnitude and angle of each force Resant forces and moments 6 Calculate all parameters: [T], [[Q Q ], h, z, z, A, A, B, B, D D midplane strains and curvatures global and local stresses and strains 12 Add new layer NO 11 Use TsaiWu failure criterion and find SR 10 Change angles YES Can SR be improved 9 NO 7 Use TsaiWu failure criterion and find SR 8 Is SR within acceptable limits YES 13 Output angles Figure 12. Flowchart describing the FibreAngleOutput program. were input into the FibreAngleOutput program. The output of the program is shown in Figure 13. It can be seen from Figure 13 that the number of layers is the same as when the eample was analysed by the Conventional Approach program; however, the fibre angles are different. Here the required angles are 49, 79 and 49 instead of the previous 0, 30 and 45. Further the SR values are all between 1 and 1.2 indicating no failure or overdesign. The new fibre angles (49, 79 and 49 ) along with the material properties, material limits and loading conditions in Table 1 were then input into the Conventional Approach program. The resing SR values were eactly the same as in Figure 13. Further, the local stresses of the new laminate, shown in Figure 14, was compared with the local stresses of the earlier laminate, shown in Figure 10. It can be seen that the local stresses in Figure 14 are constant through the thickness of each layer. This shows that the stresses were evenly distributed and not varied through the thickness of each layer. Previously the SR value on the first layer was less than 1 (Figure 11) and lower than the other two layers indicating earliest failure. However with the new layup, the SR value has increased to a value greater than one. This means that the first layer is now capable of carrying a higher load and this is evident by the values for the local stresses. The previous value at the top of the first layer was 33.5 MPa (Figure 10), and the new value is 75.7 MPa (Figure 14). This clearly demonstrates the higher load bearing capability of the new laminate. Similar trends may be seen from the other positions and from the other two layers.
10 A. RAMSAROOP ET AL. 913 Figure 13. Output of FibreAngleOutput program with Table 1 as input. Figure 14. Local stresses for laminate with angles of 49, 79, and 49. It was then decided to increase the loading conditions of the 49, 79 and 49 laminate to determine whether an increase in load will res in failure. The applied loads were increased by 10% and the resing SR values are shown in Figure 15. It can clearly be seen that all the SR values for all the layers were less than 1. An increase in loading resed in failure and therefore it may be deduced that the FibreAngleOutput program optimally designed the composite laminate for the loading conditions in Table 1. This further implies a saving in material cost as there would be no etra material used because of overdesigning.
11 914 A. RAMSAROOP ET AL. Figure 15. SR ratios for 49, 79 and 49 laminate with 10% increase in loading Finite Element Analysis For further verification of the computational ress, it was decided to perform finite element analyses on the laminates eamined in the Conventional Approach program and the FibreAngleOutput program. The package used for the analysis was MSC Patran/Nastran Two finite element models were setup, and both models represented a flat composite plate with material properties, material limits and loading conditions from Table 1. The first model had the same fibre layup that was used in the eample for the Conventional Approach program, that is, 0, 30, and 45. The analysis was run and the resing fringe plots of the stress components of each layer were plotted. These plots are shown in Figure 16. The stress plots from the finite element package corresponds to the local stresses eperienced by a laminate, in particular the stresses occurring at the middle of each layer. Comparing the stress values in Figure 16 with the stresses incurred at the middle of each layer in either Figure 6 or Figure 10, it can be seen that the values are eactly the same. This implies that the model was correctly setup and that it may be used to evaluate local stresses of laminates designed with the FibreAngle Output program. The second model was setup and was similar to the first model in every aspect ecept for the fibre layup. This model had the new fibre layup (49, 79, and 49 ) that was determined by the FibreAngleOutput program. The fringe plots of the stress components from this analysis are shown in Figure 17. Here it is also evident that the values in the plots eactly correspond to the stress values at the middle of each layer in Figure 14. This verifies the above ress from the FibreAngle Output program and supports the conclusion that the program optimally designed the composite laminate, with the fibre layup of 49, 79 and 49, for the loading conditions in Table Conclusions A MATLAB script file was generated that uses the conventional approach in the design of composite laminates. The inputs are the material properties, material limits, number of fibre layers, and the fibre orientation and thickness of each layer as well as the loading conditions. These values are then used in the governing equations, based on Hooke s law for twodimensional unidirectional laminates, to determine the global and local stresses and strains. The local stresses are compared to allowable limits via the TsaiWu failure theory. The ress from this program were compared to manually calculated eamples in the various tets [2,3] and it was found that they were eactly comparable. The above program required much guesswork in choosing inputs and was therefore inadequate to design composite laminates. Hence it was adapted to take material properties, material limits and the loading conditions as inputs. The necessary calculations were performed and the optimum number of fibre layers required as well
12 A. RAMSAROOP ET AL. 915 Figure 16. Fringe plots from Patran showing stress components for 0, 30, and 45 laminate. Figure 17. Fringe plots from Patran showing stress components for 49, 79, and 49 laminate.
13 916 A. RAMSAROOP ET AL. as the fibre angle of each layer was determined. These outputs were input into the Conventional Approach program in order to verify the ress. In each case the resing composite structure did not fail. The eample used showed that the FibreAngleOutput program optimally designed the composite laminate for the given loading conditions. Finite element analyses were conducted to verify this conclusion. The use of these programs will greatly reduce the design time of composite structures as the numerous computations are completed in a fraction of the time that it would take if done manually. The designer merely has to run the FibreAngleOutput program, and view the number of layers required and the fibre angle for each layer. The program will also aid in reducing material costs. Presently the program is limited to flat unidirectional structures but work is underway to etend it to three dimensions. There is no limit on the type of composite material as far as the matri and fibre reinforcement is concerned. 5. References [1] S. K. Mazumdar, Composite Manufacturing: Materials, Product, and Process Engineering, CRC Press LLC, Boca Raton, [2] A. K. Kaw, Mechanics of Composite Materials, CRC Press LLC, Boca Raton, [3] C. T. Herakovich, Mechanics of Fibrous Materials, John Wiley & Sons Inc., Hoboken, [4] R. M. Christensen, Mechanics of Composite Materials, Dover Publications, New York, [5] M. Akbulut and F. O. Sonmez, Optimum Design of Composite Laminates for Minimum Thickness, Computers and Structures, Vol. 86, No , 2008, pp [6] K. Sivakumar, N. G. R. Iyengar and K. Deb, Optimum Design of Laminated Composite Plates with Cutouts Using a Genetic Algorithm, Composite Structures, Vol. 42, No. 3, 1998, pp [7] S. A. Barakat and G. A. AbuFarsakh, The Use of an EnergyBased Criterion to Determine Optimum Configurations of Fibrous Composites, Composite Science and Technology, Vol. 59, No. 12, 1999, pp [8] P. Kere, M. Lyly and J. Koski, Using Micriterion Optimization for Strength Design of Composite Laminates, Composite Structures, Vol. 62, No. 34, 2003, pp [9] C. H. Park, W. I. Lee, W. S. Han and A. Vautrin, Weight Minimization of Composite Laminated Plates with Miple Constraints, Composite Science and Technology, Vol. 63, No. 7, 2003, pp [10] MediaWiki, MATLAB, wiki/matlab [11] R. V. Dukkipati, MATLAB for Mechanical Engineers, New Age International (P) Limited, New Delhi, [12] G. Z. Voyiadjis and P. I. Kattan, Mechanics of Composite Materials with MATLAB, Springer Netherlands, Dordrecht, [13] A. Gilat, MATLAB: An Introduction with Applications, John Wiley & Sons Inc., Hoboken, [14] B. D. Hahn and D. T. Valentine, Essential MATLAB for Engineers and Scientists, ButterworthHeinemann, Rome, 2007.
QUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationStacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous Orthotropic Laminates.
49th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials 710 April 2008, Schaumburg, IL AIAA 20081940 Stacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More information3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture,
3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture, 09.21.07 1. In the beam considered in PS1, steel beams carried the distributed weight of the rooms above. To reduce stress on the beam, it
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationOutline. Organization. Stresses in Beams
Stresses in Beams B the end of this lesson, ou should be able to: Calculate the maimum stress in a beam undergoing a bending moment 1 Outline Curvature Normal Strain Normal Stress Neutral is Moment of
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationModeling of the Bending Stiffness of a Bimaterial Beam by the Approximation of OneDimensional of Laminated Theory
. FloresDomínguez Int. Journal of Engineering Research and Applications RESEARCH ARTICLE OPEN ACCESS odeling of the Bending Stiffness of a Bimaterial Beam by the Approimation of OneDimensional of Laminated
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationDesign of Automobile Driveshaft using Carbon/Epoxy and Kevlar/Epoxy Composites
American Journal of Engineering Research (AJER) eissn : 23200847 pissn : 23200936 Volume02, Issue10, pp173179 www.ajer.org Research Paper Open Access Design of Automobile Driveshaft using Carbon/Epoxy
More informationKirchhoff Plates: Field Equations
20 Kirchhoff Plates: Field Equations AFEM Ch 20 Slide 1 Plate Structures A plate is a three dimensional bod characterized b Thinness: one of the plate dimensions, the thickness, is much smaller than the
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationThe stiffness tailoring of megawatt wind turbine
IOP Conference Series: Materials Science and Engineering OPEN ACCESS The stiffness tailoring of megawatt wind turbine To cite this article: Z M Li et al 2013 IOP Conf. Ser.: Mater. Sci. Eng. 52 052008
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationLinear plate bending and laminate theory
Linear plate bending and laminate theor 4M: Design Tools Eindhoven Universit of Technolog Linear plate bending A plate is a bod of which the material is located in a small region around a surface in the
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationANALYSIS OF TAPERED LAMINATED COMPOSITE TUBES UNDER TENSION AND TORSION CHETHANA SHANKARA RAO. Presented to the Faculty of the Graduate School of
ANALYSIS OF TAPERED LAMINATED COMPOSITE TUBES UNDER TENSION AND TORSION by CHETHANA SHANKARA RAO Presented to the Faculty of the Graduate School of The University of Teas at Arlington in Partial Fulfillment
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 4 Pure Bending
EA 3702 echanics & aterials Science (echanics of aterials) Chapter 4 Pure Bending Pure Bending Ch 2 Aial Loading & Parallel Loading: uniform normal stress and shearing stress distribution Ch 3 Torsion:
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationUSING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE
Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationSERVICEABILITY OF BEAMS AND ONEWAY SLABS
CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach  Fifth Edition Fifth Edition SERVICEABILITY OF BEAMS AND ONEWAY SLABS A. J. Clark School of Engineering Department of Civil
More informationThe Initiation and Growth of Delaminations Induced by Matrix Microcracks in Laminated Composites
International Journal of Fracture, 57, 1 4 199. The Initiation and Growth of Delaminations Induced by Matri Microcracks in aminated Composites J. A. NAIRN and S. HU Department of Materials Science and
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationNumerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints
THEORETICAL & APPLIED MECHANICS LETTERS 1, 041005 (2011) Numerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints M. R. Khoshravan,
More informationMaterials: engineering, science, processing and design, 2nd edition Copyright (c)2010 Michael Ashby, Hugh Shercliff, David Cebon.
Modes of Loading (1) tension (a) (2) compression (b) (3) bending (c) (4) torsion (d) and combinations of them (e) Figure 4.2 1 Standard Solution to Elastic Problems Three common modes of loading: (a) tie
More informationMECHANICS OF MATERIALS
00 The McGrawHill Companies, Inc. All rights reserved. T Edition CHAPTER MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Teas Tech Universit
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationStability Analysis of a Plane, Rectangular, Boron epoxy Laminated Plate Basing on Strength Properties Determined by Different Methods
Mechanics and Mechanical Engineering Vol. 15, No. 2 (2011) 161 181 c Technical University of Lodz Stability Analysis of a Plane, Rectangular, Boron epoxy Laminated Plate Basing on Strength Properties Determined
More informationEffects of geometry and properties of fibre and matrix on overall. composite parameters
Int. Journal of Applied Sciences and ngineering Research, ol. 3, Issue 4, 2014 www.ijaser.com 2014 by the authors Licensee IJASR Under Creative Commons License 3.0 editorial@ijaser.com Research article
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationAn Evaluation and Comparison of Models for Maximum Deflection of Stiffened Plates Using Finite Element Analysis
Marine Technology, Vol. 44, No. 4, October 2007, pp. 212 225 An Evaluation and Comparison of Models for Maximum Deflection of Stiffened Plates Using Finite Element Analysis Lior Banai 1 and Omri Pedatzur
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationFEM Modeling of a 3D Printed Carbon Fiber Pylon
FEM Modeling of a 3D Printed Carbon Fiber Pylon I. López G.*, B. Chiné, and J.L. León S. Costa Rica Institute of Technology, School of Materials Science and Engineering, Cartago, Costa Rica *Corresponding
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationFinite Element Modeling of an Aluminum Tricycle Frame
Finite Element Modeling of an Aluminum Tricycle Frame A. Rodríguez, B. Chiné*, and J. A. Ramírez Costa Rica Institute of Technology, School of Materials Science and Engineering, Cartago, Costa Rica *Corresponding
More informationAnalysis and Optimization of a Hybrid Fan Blade
Analysis and Optimization of a Hybrid Fan Blade Permas Users Conference 27.04.06 28.04.06 Strassbourg DLR German Aerospace Center, Stuttgart Institute of Structures and Design J. Ehrmanntraut, F. Kocian,
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationREPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
More informationMechanics of Materials MENG 270 Fall 2003 Exam 3 Time allowed: 90min. Q.1(a) Q.1 (b) Q.2 Q.3 Q.4 Total
Mechanics of Materials MENG 70 Fall 00 Eam Time allowed: 90min Name. Computer No. Q.(a) Q. (b) Q. Q. Q.4 Total Problem No. (a) [5Points] An air vessel is 500 mm average diameter and 0 mm thickness, the
More informationCode_Aster. Calculation algorithm of the densities of reinforcement
Titre : Algorithme de calcul des densités de ferraillage Date : 05/08/2013 Page : 1/11 Calculation algorithm of the densities of reinforcement Summary: One presents the calculation algorithm of the densities
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationAfter lecture 16 you should be able to
Lecture 16: Design of paper and board packaging Advanced concepts: FEM, Fracture Mechanics After lecture 16 you should be able to describe the finite element method and its use for paper based industry
More informationL e c t u r e. D r. S a s s a n M o h a s s e b
The Scaled smteam@gmx.ch Boundary Finite www.erdbebenschutz.ch Element Method Lecture A L e c t u r e A1 D r. S a s s a n M o h a s s e b V i s i t i n g P r o f e s s o r M. I. T. C a m b r i d g e December
More informationSIMULATION OF PLANE STRAIN FIBER COMPOSITE PLATES IN BENDING THROUGH A BEM/ACA/HM FORMULATION
8 th GRACM International Congress on Computational Mechanics Volos, 12 July 15 July 2015 SIMULATION OF PLANE STRAIN FIBER COMPOSITE PLATES IN BENDING THROUGH A BEM/ACA/HM FORMULATION Theodore V. Gortsas
More informationELASTOPLASTIC STEEL BEAM BENDING ANALYSIS BY USING ABAQUS
11 ELASTOPLASTIC STEEL BEAM BENDING ANALYSIS BY USING ABAQUS Biswajit Jena * * Corresponding author: biswa.tech88@gmail.com Abstract: In recent years tremendous efforts have been made in development of
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More information2D damping predictions of fiber composite plates: Layup effects
Available online at www.sciencedirect.com Composites Science and Technology 68 (2008) 727 733 COMPOSITES SCIENCE AND TECHNOLOGY www.elsevier.com/locate/compscitech 2D damping predictions of fiber composite
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationA review on the mechanical behaviour of curvilinear fibre composite laminated panels
A review on the mechanical behaviour of curvilinear fibre composite laminated panels Pedro Ribeiro, Hamed Ahavan IDMEC/DEMec, Faculdade de Engenharia, Universidade do Porto Porto, Portugal Andrzej Teter,
More informationAPPLICATION OF ISOTENSOIDBASED CROSS SECTIONS TO FILAMENTWOUND TOROIDAL PRESSURE VESSELS
APPLICATION OF ISOTENSOIDBASED CROSS SECTIONS TO FILAMENTWOUND TOROIDAL PRESSURE VESSELS L. Zu, S. Koussios and A. Beukers Design and Production of Composite Structures, Faculty of Aerospace Engineering
More informationEXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS
EXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS Kevin L. Peil +, Ever J. Barbero +, Eduardo M. Sosa* + Department of Mechanical and Aerospace Engineering, West Virginia University (WVU), Morgantown,
More informationUSE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION ARJUN KOTHIDAR
USE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION By ARJUN KOTHIDAR A thesis submitted in partial fulfillment of the requirements for the degree
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationExperimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 pebbles
Experimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 s D. Aquaro 1 N. Zaccari ABSTRACT Dipartimento di Ingegneria Meccanica Nucleare e della Produzione University of Pisa (Italy)
More informationFINITE ELEMENT ANALYSIS OF A LAYERED COMPOSITE CYLINDER USING THE CONNECTION BETWEEN THE MACRO AND MICROSTRUCTURE
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationQuestion 1. Ignore bottom surface. Solution: Design variables: X = (R, H) Objective function: maximize volume, πr 2 H OR Minimize, f(x) = πr 2 H
Question 1 (Problem 2.3 of rora s Introduction to Optimum Design): Design a beer mug, shown in fig, to hold as much beer as possible. The height and radius of the mug should be not more than 20 cm. The
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationFinite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras. Module  01 Lecture  11
Finite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras Module  01 Lecture  11 Last class, what we did is, we looked at a method called superposition
More informationMECHANICS OF MATERIALS
Fifth SI Edition CHTER 1 MECHNICS OF MTERILS Ferdinand. Beer E. Russell Johnston, Jr. John T. DeWolf David F. Mazurek Introduction Concept of Stress Lecture Notes: J. Walt Oler Teas Tech University Contents
More information3D Compression Molding
Autodesk Simulation Moldflow Insight 2014 3D Compression Molding Executive summary In this work, the simulation results from a program developed for the threedimensional analysis of compression molding
More informationUnified Quiz M4 May 7, 2008 M  PORTION
9:0010: 00 (last four digits) 32141 Unified Quiz M4 May 7, 2008 M  PORTION Put the last four digits of your MIT ID # on each page of the exam. Read all questions carefully. Do all work on that question
More informationME 323 Examination #2
ME 33 Eamination # SOUTION Novemer 14, 17 ROEM NO. 1 3 points ma. The cantilever eam D of the ending stiffness is sujected to a concentrated moment M at C. The eam is also supported y a roller at. Using
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationFiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens
Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: www.astm.org FiniteElement
More informationEnergy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses
International Journal of Adhesion & Adhesives 20 (1999) 59 70 International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing
More informationSpherical Pressure Vessels
Spherical Pressure Vessels Pressure vessels are closed structures containing liquids or gases under essure. Examples include tanks, pipes, essurized cabins, etc. Shell structures : When essure vessels
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationEXPERIMENTAL STUDY ON YOUNG S MODULUS E OF A POLYMER COMPOSITE REINFORCED BY NANO TITANIUM DIOXIDE PARTICLES
Vietnam Journal of Mechanics, VAST, Vol. 34, No. (202), pp. 9 25 EXPERIMENTAL STUDY ON YOUNG S MODULUS E OF A POLYMER COMPOSITE REINFORCED BY NANO TITANIUM DIOXIDE PARTICLES Nguyen Dinh Duc, Dinh Khac
More informationLab Exercise #3: Torsion
Lab Exercise #3: Prelab assignment: Yes No Goals: 1. To evaluate the equations of angular displacement, shear stress, and shear strain for a shaft undergoing torsional stress. Principles: testing of round
More informationImplications of failure criteria choices on the rapid concept design of composite grillage structures using multiobjective optimisation
Noname manuscript No. (will be inserted by the editor) Implications of failure criteria choices on the rapid concept design of composite grillage structures using multiobjective optimisation A.J.Sobey
More information